Intergrowth Compounds in the Zn-Rich Zn−Pd System: Toward 1D Quasicrystal Approximants
Gourdon, Olivier; Miller, Gordon J.; Chemistry of Materials 18 (2006) 1848–; doi:10.1021/cm0526415

data_4001517
_publ_section_title
;
 Intergrowth Compounds in the Zn-Rich Zn&#x2212;Pd System:&#x00A0; Toward
 1D Quasicrystal Approximants
;
_journal_issue                   7
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1848
_journal_paper_doi               10.1021/cm0526415
_journal_volume                  18
_journal_year                    2006
_chemical_formula_sum            'Pd2.352 Zn10.648'
_chemical_formula_weight         946.4
_chemical_name_systematic        ' ?'
_space_group_IT_number           217
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.0906
_cell_length_b                   9.0906
_cell_length_c                   9.0906
_cell_volume                     751.238
_computing_publication_material  '(Jana2000; Petricek and Dusek, 2000)'
_computing_structure_refinement  '(Jana2000; Petricek and Dusek, 2000)'
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.99
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0379
_diffrn_reflns_av_sigmaI/netI    0.0189
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            3239
_diffrn_reflns_theta_full        28.18
_diffrn_reflns_theta_max         28.18
_diffrn_reflns_theta_min         3.17
_exptl_absorpt_coefficient_mu    41.530
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  1.000
_exptl_absorpt_correction_type   analytical
_exptl_crystal_density_diffrn    8.9807
_exptl_crystal_F_000             1710
_refine_diff_density_max         0.53
_refine_diff_density_min         -0.76
_refine_ls_extinction_coef       0.0259(15)
_refine_ls_extinction_method
'B-C type 1 Lorentzian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.33
_refine_ls_goodness_of_fit_ref   1.33
_refine_ls_number_parameters     19
_refine_ls_number_reflns         200
_refine_ls_R_factor_all          0.0130
_refine_ls_R_factor_gt           0.0130
_refine_ls_shift/su_max          0.0185
_refine_ls_shift/su_mean         0.0064
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/\s^2^(I)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0268
_refine_ls_wR_factor_ref         0.0268
_reflns_number_gt                200
_reflns_number_total             200
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            cm0526415si20051130_114748.cif
_cod_data_source_block           (I)
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Analytical' changed to
'analytical' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        751.2382
_cod_original_sg_symbol_Hall     'I -4;2;3'
_cod_database_code               4001517